distinction is made between thin films and solvent-based methods. Solvothermal synthesis can be carried out conventionally in a teflon reactor in a convection oven or in glass reactors in a microwave oven (high-throughput microwave synthesis). The use of a microwave oven changes, in part dramatically, the reaction parameters. In addition to solvothermal synthesis, there have been advances in using supercritical fluid as a solvent in a continuous flow reactor. Supercritical water was first used in 2012 to synthesize copper and nickel-based MOFs in just seconds. In 2020, supercritical carbon dioxide was used in a continuous flow reactor along the same time scale as the supercritical water-based method, but the lower critical point of carbon dioxide allowed for the synthesis of the zirconium-based MOF UiO-66. High-throughput solvothermal synthesis In high-throughput solvothermal synthesis, a solvothermal reactor with (eg) 24 cavities for teflon reactors is used. Such a reactor is sometimes referred to as a multiclav. The reactor block or reactor insert is made of stainless steel and contains 24 reaction chambers, which are arranged in four rows. With the miniaturized teflon reactors, volumes of up to 2 mL can be used. The reactor block is sealed in a stainless steel autoclave; for this purpose, the filled reactors are inserted into the bottom of the reactor, the teflon reactors are sealed with two teflon films and the reactor top side is put on. The autoclave is then closed in a hydraulic press. The sealed solvothermal reactor can then be subjected to a temperature-time program. The reusable teflon film serves to withstand the mechanical stress, while the disposable teflon film seals the reaction vessels. After the reaction, the products can be isolated and washed in parallel in a vacuum filter device. On the filter paper, the products are then present separately in a so-called sample library and can subsequently be characterized by automated X-ray powder diffraction. The informations obtained are then used to plan further syntheses. Pseudomorphic replication Pseudomorphic mineral replacement events occur whenever a mineral phase comes into contact with a fluid with which it is out of equilibrium. Re-equilibration will tend to take place to reduce the free energy and transform the initial phase into a more thermodynamically stable phase, involving dissolution and reprecipitation subprocesses. Inspired by such geological processes, MOF thin films can be grown through the combination of atomic layer deposition (ALD) of aluminum oxide onto a suitable substrate (e.g.